Transparent conductive carbon nanotube ï¬lms - SMF conductive carbon nanotube...
Embed Size (px)
Transcript of Transparent conductive carbon nanotube ï¬lms - SMF conductive carbon nanotube...
RESEARCH Revista Mexicana de Fsica 63 (2017) 439-447 SEPTEMBER-OCTOBER 2017
Transparent conductive carbon nanotube films
S. Muhla, R. Aguilar Osoriob and U.A. Martnez HuitlebaInstituto de Investigaciones en Materiales, Universidad Nacional Autonoma de Mexico,
Coyoacan, 04510, Ciudad de Mexico.bInstituto Politecnico Nacional. SEPI ESIME Zac, UPALM.
Edificio 5, 3er. Piso Col. Lindavista, 07738, Ciudad de Mexico.e-mail: firstname.lastname@example.org
Received 9 December 2016; accepted 15 June 2017
This work presents the results of a study of the fabrication of multiwall carbon nanotubes (MWCNTs) by chemical vapour deposition (CVD),the purification and the development of transparent conductors films (TCFs) using these nanotubes. The as produced MWCNTs had someimpurities due the CVD method including small amounts of the iron catalyst, amorphous carbon and hydrocarbon residues from the organicprecursors. These impurities have been reported to be detrimental to both the electrical and optical properties of the TCFs. For this reasonthe purification of the nanotubes was studied using 3 different techniques. The three methods involved; A) selective oxidation in air of theMWCNTs followed by a hydrochloric acid solution etch to remove the iron, B) a selective oxidation using H2O2 followed by the hydrochloricacid etch treatment, and C) an oxidation-etch procedure using a mixture of H2O2 and hydrochloric acid. The best result results were obtainedusing the combined H2O2 and hydrochloric acid treatment. With this method MWCNTs were obtained with a purity of up to 94%. Thepurified MWCNTs were dispersed in solutions of different solvents without surfactant. Thin films of MWCNT were fabricated using acombined spray and spin coating technique, which produced a uniform deposit of controllable thickness. Either a transparent nitrocellulose-based varnish or acrylic was used to fix the film to the glass substrate. Both the optical transparency and the electrical square resistivity ofthe samples were measured by spectrophotometry and standard electrical techniques, respectively. Our results were similar to those of othergroups in that the transparency was almost inversely proportional to the resistivity.
Keywords: Transparent conductive films; carbon nanotubes; carbon nanotube films; thin films
PACS: 78.67.Ch; 81.07.De; 81.15.Rs
Transparent conducting films, TCFs, are electrically conduc-tive in thin films they are widely used as a component ofsolar cells and many other optical electronic devices. Suchfilms have been developed from different materials, includ-ing indium tin oxide, (ITO), tin oxide (SnO2), and zinc oxide(ZnO). According to several researchers [1-10] ITO is one ofthe most widely used transparent conducting oxides. Its pop-ularity is mainly due to two good properties, one, its electricalconductivity, and the other, its optical transparency, in addi-tion, it is ease to deposit as a thin film. However, ITO is themost expensive material because of the process of fabricationand the limited world reserves of indium. Recently, interestin developing TCFs on flexible materials has increased, andfor this ITO is not viable because it is fragile and tends tobreak. As consequence, in the last few years the use of car-bon nanotubes, CNTS, based TCFs have increased. This is inpart because of the reduced cost, and higher flexibility.
There are several methods for manufacturing the CNTsincluding: electric arc discharge, laser evaporation/ablationand chemical vapour deposition (CVD). The oldest methodfor the carbon nanotube manufacturing is the electric arc dis-charge [11-14]. This method was used in the early sixtiesby R. Bacon  for the synthesis of carbon fibres, that theycalled whiskers. In 1990 Kratschmer and Huffman used themethod [16-17] to obtain fullerenes, and later the method
was improved and extended for the synthesis of multiwall(MWCNT) and single wall (SWNT) carbon nanotubes.
The arc-discharge and laser-ablation techniques have lim-itations and purification of the product must be carried outto eliminate impurities. Another alternative is the chemicalvapour deposition (CVD), with this method the nanotubes areproduced by the decomposition of a carbon-containing gas inthe presence of a catalyst. CVD method [18-21] is widelyused to manufacture nanotubes because it is possible to ob-tain aligned CNTs of high purity, high density and in eco-nomical viable quantities. This method was originally devel-oped in the 1960s and 1970s and has been successfully usedfor the production of carbon fibres and carbon nanofibres.
In this paper the fabrication and characterization of thetransparent conducting films based on MWCNTs is pre-sented.
2.1. Fabrication, purification and characterization ofthe MWCNTs
To develop the transparent conducting films (TCF) theMWCNTs were fabricated using a CVD reaction of camphorand ferrocene in a nitrogen atmosphere, characterized and pu-rified using various procedures [22,26,27].
440 S. MUHL, R. AGUILAR OSORIO AND U.A. MARTINEZ HUITLE
FIGURE 1. A schematic drawing of the gas and precursor vapour mixture injector.
The best experimental conditions had been established inprevious studies and consisted of the use of a 38.4 mm inte-rior diameter tube furnace temperature at 850C, an evapo-ration temperature of 215C for the 95 wt% camphor (96%Sigma-Aldrich) with 5 wt% ferrocene (98% Sigma-Aldrich)precursor mixture and a nitrogen (99.99% purity) gas flow of100 ml/min at atmospheric pressure.
The MWCNTs were grown on 1.5 3 cm pieces ofcleaned crystalline silicon, but the deposit formed on the in-terior wall of the alumina furnace tube was also collectedand used. The MWCNT deposit on the silicon was mechan-ically removed for the characterization and the purificationprocesses. One significant difference of our CVD setup toother reported systems is that a precursor injector was devel-oped and used to prevent the condensation of the precursorvapour mixture before it was introduced to the hot region ofthe furnace, see Fig. 1.
The injector and evaporation sections of the system canbe heated independentally and tempertures of 225C and215C, respectively, were used in these experiments. Thelength of the injector was sufficient to ensure that the exitis at a furnace temperature greater than 225C, in this waythe precurs vapour is always at a temperature greater than itsboiling point (175C). The concentric outer tube, OT, andthe inner thermal barrier tube ensured that the vacuum con-nector is sufficiently cool, < 60C, to not suffer damagedduring the experiment. The use of the injector assembly wasfound to significantly increase the production of MWCNTsand permit much better reproducibility in the experiments.
The collected material contained various types of impuri-ties which could degrade the electrical and optical propertiesof the CNTs films. Therefore, we studied the purification ofthe deposit using three chemical procedures: a gas phase se-lective oxidation and two types of liquid phase selective ox-
idation. Initially, the MWCNTs samples were dispersed ineither acetone or DI water (for the gas or liquid phase, re-spectively) and subjected to 60 minutes of room temperatureultrasonic bath agitation to separate the large a-C particlesfrom the MWCNTs. Yu et al.  reported that longer timescould cause significant fracture of the CNTs.
For the first purification method the acetone-MWCNTsample was dripped on a 70C quartz plate to produce a drysolid deposit. This was then heated to 520C in a 40 ml/minflow of air for 0.5, 1.5, 3.5 or 5 hrs. The material was then me-chanical removed from the plates and mixed with hydrochlo-ric acid. The mixture was placed in an ultrasonic bath for1 min then left for 1 hr. to ensure as complete as possibleremoval of the iron particles. Finally, the majority of the acidon top of the precipitated MWCNTs was removed, DI waterwas added and again the excess liquid was removed after theMWCNTs had settled in the bottom of the recipient. Thisprocedure was repeated three times after the sediment haddried, then ethanol was added and the agitated mixture wasdeposited on glass plates at 70C, followed by a 30 min treat-ment in air at 120C, this formula was used to make fully drysamples for the various characterization procedures.
The second purification method consisted of mixing25 ml of the water-MWCNT sample with 160 ml of a 3.5%solution of hydrogen peroxide in DI water. This mixture wasthen subjected to ultrasonic agitation for 2 hrs. at 60C, fi-nally 100 ml of 38% HCl was added and the sample was leftfor 12 hrs. A dried solid sample was then prepared as in thecase of the previous gas phase oxidation.
The third procedure was similar to the second processbut 40 ml of the peroxide solution was added simultaneouslywith 20 ml of HCl. A dried solid sample was then preparedas for the other procedures.
Rev. Mex. Fis. 63 (2017) 439-447
TRANSPARENT CONDUCTIVE CARBON NANOTUBE FILMS 441
Finally for all the sample types, the obtained material washeat treated at 340C for 30 m.
The MWCNT samples were characterised using thermo-gravimetric analysis (TGA) performed in air with a flow rateof 40 ml/min using a heating rate of 10C/min from 25 to800C, transmission electron microscopy (TEM), scanningelectron microscope (SEM), energy-dispersion spectrometry(EDS), Raman spectroscopy, optical microscopy and X-raydiffraction.
2.2. Fabrication of the transparent conducting films
The starting point for fabrication the transparent conductingfilms (TCFs) based on the MWCNTs was the preparationof colloidal inks to facilitate the dispersion of the nanotubeswhen the glass substrates were spray coated. Three types ofinks were used:
1) Isopropyl alcohol (IPA) (99.8% pure) with between0.0